#------------------------------------------------------------------------------
#$Date: 2016-02-20 18:35:30 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176787 $
#$URL: svn://www.crystallography.net/cod/cif/2/21/14/2211415.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2211415
loop_
_publ_author_name
'Bo Liu'
'Shi Zhou'
'Chuan-Bi Li'
'Hong-Gang Zhang'
_publ_section_title
;
 Bis(guanidinium) hexahydroxooctadecaoxodisodiohexamolybdonickelate
 decahydrate
;
_journal_coeditor_code           HB2182
_journal_issue                   12
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              m3185
_journal_page_last               m3187
_journal_paper_doi               10.1107/S160053680604503X
_journal_volume                  62
_journal_year                    2006
_chemical_formula_iupac          '(C H6 N3)2 [Na2 Ni (O H)6 Mo6 O18] , 10H2 O'
_chemical_formula_moiety         '2C H6 N3 + , H14 Mo6 Na2 Ni O28 2- , 6H2 O'
_chemical_formula_sum            'C2 H38 Mo6 N6 Na2 Ni O34'
_chemical_formula_weight         1370.69
_chemical_name_systematic
;Bis(guanidinium) hexahydroxooctadecaoxodisodiohexamolybdonickelate
 decahydrate
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL97
_cell_angle_alpha                90.00
_cell_angle_beta                 114.918(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   25.2247(9)
_cell_length_b                   11.6583(4)
_cell_length_c                   13.7668(5)
_cell_measurement_reflns_used    5347
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.05
_cell_measurement_theta_min      1.80
_cell_volume                     3671.6(3)
_computing_cell_refinement       'SAINT (Bruker, 2002)'
_computing_data_collection       'SMART (Bruker, 2002)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  SHELXTL
_computing_structure_refinement  SHELXTL
_computing_structure_solution    'SHELXTL (Bruker, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.984
_diffrn_measured_fraction_theta_max 0.984
_diffrn_measurement_device_type  'Bruker SMART APEXII CCD area-detector'
_diffrn_measurement_method       'ω and φ'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0174
_diffrn_reflns_av_sigmaI/netI    0.0206
_diffrn_reflns_limit_h_max       30
_diffrn_reflns_limit_h_min       -31
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            9516
_diffrn_reflns_theta_full        26.01
_diffrn_reflns_theta_max         26.01
_diffrn_reflns_theta_min         2.78
_exptl_absorpt_coefficient_mu    2.622
_exptl_absorpt_correction_T_max  0.630
_exptl_absorpt_correction_T_min  0.475
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2002)'
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.480
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             2664
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.18
_refine_diff_density_max         0.645
_refine_diff_density_min         -0.633
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.017
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     233
_refine_ls_number_reflns         3557
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.017
_refine_ls_R_factor_all          0.0266
_refine_ls_R_factor_gt           0.0235
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0316P)²+13.3478P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0584
_refine_ls_wR_factor_ref         0.0597
_reflns_number_gt                3275
_reflns_number_total             3557
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            hb2182.cif
_cod_data_source_block           I
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               2211415
_cod_database_fobs_code          2211415
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
Ni Ni 0.7500 0.7500 0.0000 0.01399(12) Uani d S 1
Mo Mo1 0.875219(11) 0.65271(2) 0.18571(2) 0.01685(8) Uani d . 1
Mo Mo2 0.627324(11) 0.71958(2) 0.03086(2) 0.01634(8) Uani d . 1
Mo Mo3 0.752803(11) 0.62372(2) 0.21791(2) 0.01563(8) Uani d . 1
Na Na 0.83122(6) 0.34440(12) 0.19303(11) 0.0304(3) Uani d . 1
O O1 0.78101(9) 0.60580(18) 0.08711(16) 0.0160(4) Uani d . 1
H H1 0.7719 0.5389 0.0561 0.019 Uiso d R 1
O O2 0.72033(9) 0.78138(17) 0.11499(16) 0.0151(4) Uani d . 1
H H2 0.7252 0.8473 0.1452 0.018 Uiso d R 1
O O3 0.83390(9) 0.80500(18) 0.08610(17) 0.0168(4) Uani d . 1
H H3 0.8382 0.8667 0.1147 0.020 Uiso d R 1
O O4 0.88537(10) 0.64101(18) 0.05404(18) 0.0200(5) Uani d . 1
O O5 0.82963(10) 0.69438(19) 0.26683(17) 0.0191(4) Uani d . 1
O O6 0.77292(11) 0.4850(2) 0.25988(19) 0.0258(5) Uani d . 1
O O7 0.61116(10) 0.7807(2) 0.12909(18) 0.0254(5) Uani d . 1
O O8 0.67600(9) 0.59067(18) 0.10722(18) 0.0195(4) Uani d . 1
O O9 0.89049(11) 0.5110(2) 0.22220(19) 0.0270(5) Uani d . 1
O O10 0.93650(10) 0.7243(2) 0.26786(19) 0.0317(6) Uani d . 1
O O11 0.56614(11) 0.6427(2) -0.0445(2) 0.0301(6) Uani d . 1
O O12 0.73482(10) 0.6854(2) 0.31356(18) 0.0248(5) Uani d . 1
O OW1 0.75490(12) 0.3860(2) 0.0220(2) 0.0315(6) Uani d . 1
H H1WA 0.7245 0.3661 0.0292 0.038 Uiso d R 1
H H1WB 0.7474 0.3601 -0.0385 0.038 Uiso d R 1
O OW2 0.65516(15) 0.3564(2) 0.0716(2) 0.0471(8) Uani d . 1
H H2WA 0.6636 0.4281 0.0964 0.057 Uiso d R 1
H H2WB 0.6682 0.3233 0.1355 0.057 Uiso d R 1
O OW3 0.63482(16) 0.4915(3) 0.2827(3) 0.0581(9) Uani d . 1
H H3WA 0.6255 0.5451 0.3154 0.070 Uiso d R 1
H H3WB 0.6511 0.5313 0.2470 0.070 Uiso d R 1
O OW4 0.5000 0.4497(7) 0.2500 0.113(5) Uani d S 1
H H4W 0.5300 0.4079 0.2624 0.135 Uiso d R 1
O OW5 0.5000 0.6753(7) 0.2500 0.142(4) Uani d S 1
H H5W 0.4920 0.6310 0.2969 0.171 Uiso d R 1
O OW6 0.88282(14) 0.2150(3) 0.1377(2) 0.0466(7) Uani d . 1
H H6WA 0.9182 0.2218 0.1812 0.056 Uiso d R 1
H H6WB 0.8772 0.1987 0.0761 0.056 Uiso d R 1
N N1 0.90291(13) 0.5722(3) 0.4734(2) 0.0337(7) Uani d . 1
H H1A 0.8817 0.6152 0.4205 0.040 Uiso calc R 1
H H1B 0.8887 0.5098 0.4860 0.040 Uiso calc R 1
N N2 0.98862(15) 0.5344(3) 0.6167(3) 0.0459(9) Uani d . 1
H H2A 0.9738 0.4725 0.6286 0.055 Uiso calc R 1
H H2B 1.0241 0.5528 0.6577 0.055 Uiso calc R 1
N N3 0.97935(16) 0.6976(3) 0.5166(3) 0.0491(10) Uani d . 1
H H3A 0.9586 0.7413 0.4640 0.059 Uiso calc R 1
H H3B 1.0148 0.7161 0.5576 0.059 Uiso calc R 1
C C1 0.95669(15) 0.6017(3) 0.5347(3) 0.0281(8) Uani d . 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O1 Ni O1 7_665 . 180.0 n
O1 Ni O3 7_665 7_665 82.51(8) n
O1 Ni O3 . 7_665 97.49(8) n
O1 Ni O3 7_665 . 97.49(8) n
O1 Ni O3 . . 82.51(8) n
O3 Ni O3 7_665 . 180.0 n
O1 Ni O2 7_665 7_665 82.31(8) n
O1 Ni O2 . 7_665 97.69(8) n
O3 Ni O2 7_665 7_665 97.00(8) n
O3 Ni O2 . 7_665 83.00(8) n
O1 Ni O2 7_665 . 97.69(8) n
O1 Ni O2 . . 82.31(8) n
O3 Ni O2 7_665 . 83.00(8) n
O3 Ni O2 . . 97.00(8) n
O2 Ni O2 7_665 . 180.0 n
O10 Mo1 O9 . . 104.36(12) n
O10 Mo1 O4 . . 102.42(11) n
O9 Mo1 O4 . . 95.95(10) n
O10 Mo1 O5 . . 94.94(11) n
O9 Mo1 O5 . . 100.56(10) n
O4 Mo1 O5 . . 152.24(9) n
O10 Mo1 O3 . . 94.42(11) n
O9 Mo1 O3 . . 159.65(10) n
O4 Mo1 O3 . . 72.00(8) n
O5 Mo1 O3 . . 85.34(8) n
O10 Mo1 O1 . . 162.32(11) n
O9 Mo1 O1 . . 89.56(10) n
O4 Mo1 O1 . . 86.61(9) n
O5 Mo1 O1 . . 71.46(8) n
O3 Mo1 O1 . . 73.73(8) n
O11 Mo2 O7 . . 104.01(12) n
O11 Mo2 O8 . . 97.25(11) n
O7 Mo2 O8 . . 101.53(10) n
O11 Mo2 O4 . 7_665 101.26(11) n
O7 Mo2 O4 . 7_665 95.29(10) n
O8 Mo2 O4 . 7_665 151.12(9) n
O11 Mo2 O3 . 7_665 93.03(10) n
O7 Mo2 O3 . 7_665 160.42(10) n
O8 Mo2 O3 . 7_665 85.52(9) n
O4 Mo2 O3 7_665 7_665 71.62(8) n
O11 Mo2 O2 . . 163.68(10) n
O7 Mo2 O2 . . 90.21(10) n
O8 Mo2 O2 . . 71.68(8) n
O4 Mo2 O2 7_665 . 85.06(9) n
O3 Mo2 O2 7_665 . 74.53(8) n
O6 Mo3 O12 . . 105.76(11) n
O6 Mo3 O8 . . 97.66(11) n
O12 Mo3 O8 . . 100.76(10) n
O6 Mo3 O5 . . 99.89(10) n
O12 Mo3 O5 . . 95.93(10) n
O8 Mo3 O5 . . 151.44(9) n
O6 Mo3 O1 . . 91.96(10) n
O12 Mo3 O1 . . 160.64(10) n
O8 Mo3 O1 . . 84.18(9) n
O5 Mo3 O1 . . 72.91(8) n
O6 Mo3 O2 . . 162.84(10) n
O12 Mo3 O2 . . 89.82(10) n
O8 Mo3 O2 . . 71.87(8) n
O5 Mo3 O2 . . 85.27(8) n
O1 Mo3 O2 . . 73.80(7) n
OW6 Na O7 . 4_645 87.20(11) n
OW6 Na O9 . . 100.76(11) n
O7 Na O9 4_645 . 90.75(9) n
OW6 Na OW1 . . 98.03(11) n
O7 Na OW1 4_645 . 166.02(11) n
O9 Na OW1 . . 100.92(10) n
OW6 Na O12 . 4_645 87.87(11) n
O7 Na O12 4_645 4_645 85.05(9) n
O9 Na O12 . 4_645 170.22(10) n
OW1 Na O12 . 4_645 82.21(9) n
OW6 Na O6 . . 178.07(11) n
O7 Na O6 4_645 . 91.35(9) n
O9 Na O6 . . 80.53(9) n
OW1 Na O6 . . 83.09(9) n
O12 Na O6 4_645 . 90.73(9) n
Ni O1 Mo3 . . 103.18(9) n
Ni O1 Mo1 . . 101.65(9) n
Mo3 O1 Mo1 . . 96.10(8) n
Ni O1 H1 . . 119.8 n
Mo3 O1 H1 . . 112.1 n
Mo1 O1 H1 . . 120.3 n
Ni O2 Mo2 . . 100.72(8) n
Ni O2 Mo3 . . 100.70(8) n
Mo2 O2 Mo3 . . 94.95(8) n
Ni O2 H2 . . 120.7 n
Mo2 O2 H2 . . 116.2 n
Mo3 O2 H2 . . 119.1 n
Ni O3 Mo1 . . 102.09(9) n
Ni O3 Mo2 . 7_665 101.72(9) n
Mo1 O3 Mo2 . 7_665 96.26(8) n
Ni O3 H3 . . 117.2 n
Mo1 O3 H3 . . 118.8 n
Mo2 O3 H3 7_665 . 117.4 n
Mo1 O4 Mo2 . 7_665 116.68(11) n
Mo3 O5 Mo1 . . 115.66(10) n
Mo3 O6 Na . . 126.96(12) n
Mo2 O7 Na . 4_655 133.87(13) n
Mo3 O8 Mo2 . . 117.83(11) n
Mo1 O9 Na . . 133.33(13) n
Mo3 O12 Na . 4_655 132.64(13) n
Na OW1 H1WA . . 103.0 n
Na OW1 H1WB . . 131.7 n
H1WA OW1 H1WB . . 100.6 n
H2WA OW2 H2WB . . 95.6 n
H3WA OW3 H3WB . . 101.5 n
Na OW6 H6WA . . 106.1 n
Na OW6 H6WB . . 127.7 n
H6WA OW6 H6WB . . 115.3 n
C1 N1 H1A . . 120.0 n
C1 N1 H1B . . 120.0 n
H1A N1 H1B . . 120.0 n
C1 N2 H2A . . 120.0 n
C1 N2 H2B . . 120.0 n
H2A N2 H2B . . 120.0 n
C1 N3 H3A . . 120.0 n
C1 N3 H3B . . 120.0 n
H3A N3 H3B . . 120.0 n
N1 C1 N3 . . 120.9(4) n
N1 C1 N2 . . 119.0(4) n
N3 C1 N2 . . 120.1(4) n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Ni O1 . 2.021(2) y
Ni O3 . 2.045(2) y
Ni O2 . 2.049(2) y
Ni O1 7_665 2.021(2) n
Ni O3 7_665 2.045(2) n
Ni O2 7_665 2.049(2) n
Mo1 O10 . 1.701(2) y
Mo1 O9 . 1.723(2) y
Mo1 O4 . 1.939(2) y
Mo1 O5 . 1.972(2) y
Mo1 O3 . 2.217(2) y
Mo1 O1 . 2.252(2) y
Mo2 O11 . 1.707(2) y
Mo2 O7 . 1.723(2) y
Mo2 O8 . 1.945(2) y
Mo2 O4 7_665 1.948(2) y
Mo2 O3 7_665 2.227(2) y
Mo2 O2 . 2.253(2) y
Mo3 O6 . 1.720(2) y
Mo3 O12 . 1.721(2) y
Mo3 O8 . 1.933(2) y
Mo3 O5 . 1.946(2) y
Mo3 O1 . 2.207(2) y
Mo3 O2 . 2.254(2) y
Na OW6 . 2.321(3) y
Na O7 4_645 2.379(3) y
Na O9 . 2.379(3) y
Na OW1 . 2.380(3) y
Na O12 4_645 2.468(3) y
Na O6 . 2.615(3) y
O1 H1 . 0.8723 n
O2 H2 . 0.8574 n
O3 H3 . 0.8049 n
OW1 H1WA . 0.8460 n
OW1 H1WB . 0.8295 n
OW2 H2WA . 0.8948 n
OW2 H2WB . 0.8877 n
OW3 H3WA . 0.8583 n
OW3 H3WB . 0.8918 n
OW4 H4W . 0.8542 n
OW5 H5W . 0.9141 n
OW6 H6WA . 0.8430 n
OW6 H6WB . 0.8211 n
N1 C1 . 1.306(5) n
N1 H1A . 0.8600 n
N1 H1B . 0.8600 n
N2 C1 . 1.331(5) n
N2 H2A . 0.8600 n
N2 H2B . 0.8600 n
N3 C1 . 1.327(5) n
N3 H3A . 0.8600 n
N3 H3B . 0.8600 n
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
O1 H1 OW1 . 0.87 1.85 2.703(3) 167
O2 H2 O6 4_655 0.86 2.06 2.896(3) 165
O3 H3 OW3 4_655 0.80 1.94 2.722(4) 164
OW1 H1WB O12 6_565 0.83 2.00 2.822(3) 173
OW1 H1WA OW2 . 0.85 2.07 2.892(4) 165
OW2 H2WA O8 . 0.89 1.92 2.786(4) 164
OW2 H2WB O5 4_645 0.89 2.00 2.818(3) 152
OW3 H3WA OW6 4_655 0.86 2.12 2.932(4) 158
OW5 H5W OW4 . 0.91 2.24 2.630(11) 105
OW6 H6WA OW5 4_645 0.84 1.95 2.736(4) 155
OW6 H6WB OW2 7_655 0.82 1.95 2.754(4) 165
OW6 H6WA OW5 3_545 0.84 1.95 2.736(4) 155
N1 H1A O5 . 0.86 2.17 3.017(4) 168
N1 H1B O4 6_566 0.86 2.01 2.832(4) 159
N2 H2B O9 5_766 0.86 2.22 2.966(4) 145
N3 H3B O7 8_566 0.86 2.20 3.029(4) 161
N3 H3B O11 8_566 0.86 2.81 3.243(4) 113
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
O3 Ni O1 Mo3 7_665 . -81.79(9) n
O3 Ni O1 Mo3 . . 98.21(9) n
O2 Ni O1 Mo3 7_665 . -179.95(8) n
O2 Ni O1 Mo3 . . 0.05(8) n
O3 Ni O1 Mo1 7_665 . 179.02(8) n
O3 Ni O1 Mo1 . . -0.98(8) n
O2 Ni O1 Mo1 7_665 . 80.86(9) n
O2 Ni O1 Mo1 . . -99.14(9) n
O6 Mo3 O1 Ni . . 170.23(11) n
O12 Mo3 O1 Ni . . -33.3(3) n
O8 Mo3 O1 Ni . . 72.73(10) n
O5 Mo3 O1 Ni . . -90.02(10) n
O2 Mo3 O1 Ni . . -0.05(8) n
O6 Mo3 O1 Mo1 . . -86.26(10) n
O12 Mo3 O1 Mo1 . . 70.2(3) n
O8 Mo3 O1 Mo1 . . 176.24(9) n
O5 Mo3 O1 Mo1 . . 13.49(8) n
O2 Mo3 O1 Mo1 . . 103.46(8) n
O10 Mo1 O1 Ni . . 50.3(4) n
O9 Mo1 O1 Ni . . -167.28(11) n
O4 Mo1 O1 Ni . . -71.29(9) n
O5 Mo1 O1 Ni . . 91.42(10) n
O3 Mo1 O1 Ni . . 0.94(7) n
O10 Mo1 O1 Mo3 . . -54.6(3) n
O9 Mo1 O1 Mo3 . . 87.87(10) n
O4 Mo1 O1 Mo3 . . -176.14(9) n
O5 Mo1 O1 Mo3 . . -13.42(8) n
O3 Mo1 O1 Mo3 . . -103.91(9) n
O1 Ni O2 Mo2 7_665 . 82.76(9) n
O1 Ni O2 Mo2 . . -97.24(9) n
O3 Ni O2 Mo2 7_665 . 1.34(8) n
O3 Ni O2 Mo2 . . -178.66(8) n
O1 Ni O2 Mo3 7_665 . 179.95(8) n
O1 Ni O2 Mo3 . . -0.05(8) n
O3 Ni O2 Mo3 7_665 . 98.53(9) n
O3 Ni O2 Mo3 . . -81.47(9) n
O11 Mo2 O2 Ni . . 40.2(4) n
O7 Mo2 O2 Ni . . -168.83(10) n
O8 Mo2 O2 Ni . . 89.09(10) n
O4 Mo2 O2 Ni 7_665 . -73.54(9) n
O3 Mo2 O2 Ni 7_665 . -1.26(8) n
O11 Mo2 O2 Mo3 . . -61.7(4) n
O7 Mo2 O2 Mo3 . . 89.27(10) n
O8 Mo2 O2 Mo3 . . -12.81(8) n
O4 Mo2 O2 Mo3 7_665 . -175.44(9) n
O3 Mo2 O2 Mo3 7_665 . -103.16(8) n
O6 Mo3 O2 Ni . . -34.8(4) n
O12 Mo3 O2 Ni . . 169.58(11) n
O8 Mo3 O2 Ni . . -89.03(10) n
O5 Mo3 O2 Ni . . 73.61(9) n
O1 Mo3 O2 Ni . . 0.05(8) n
O6 Mo3 O2 Mo2 . . 67.1(3) n
O12 Mo3 O2 Mo2 . . -88.52(10) n
O8 Mo3 O2 Mo2 . . 12.88(8) n
O5 Mo3 O2 Mo2 . . 175.52(9) n
O1 Mo3 O2 Mo2 . . 101.96(8) n
O1 Ni O3 Mo1 7_665 . -179.00(8) n
O1 Ni O3 Mo1 . . 1.00(8) n
O2 Ni O3 Mo1 7_665 . -97.75(9) n
O2 Ni O3 Mo1 . . 82.25(9) n
O1 Ni O3 Mo2 7_665 7_665 -79.89(9) n
O1 Ni O3 Mo2 . 7_665 100.11(9) n
O2 Ni O3 Mo2 7_665 7_665 1.36(8) n
O2 Ni O3 Mo2 . 7_665 -178.64(8) n
O10 Mo1 O3 Ni . . -167.57(11) n
O9 Mo1 O3 Ni . . 35.0(3) n
O4 Mo1 O3 Ni . . 90.79(10) n
O5 Mo1 O3 Ni . . -72.96(9) n
O1 Mo1 O3 Ni . . -0.93(7) n
O10 Mo1 O3 Mo2 . 7_665 88.99(10) n
O9 Mo1 O3 Mo2 . 7_665 -68.4(3) n
O4 Mo1 O3 Mo2 . 7_665 -12.65(8) n
O5 Mo1 O3 Mo2 . 7_665 -176.40(9) n
O1 Mo1 O3 Mo2 . 7_665 -104.37(9) n
O10 Mo1 O4 Mo2 . 7_665 -74.48(15) n
O9 Mo1 O4 Mo2 . 7_665 179.37(13) n
O5 Mo1 O4 Mo2 . 7_665 52.9(3) n
O3 Mo1 O4 Mo2 . 7_665 16.17(11) n
O1 Mo1 O4 Mo2 . 7_665 90.16(12) n
O6 Mo3 O5 Mo1 . . 71.91(13) n
O12 Mo3 O5 Mo1 . . 179.09(12) n
O8 Mo3 O5 Mo1 . . -55.2(2) n
O1 Mo3 O5 Mo1 . . -17.09(10) n
O2 Mo3 O5 Mo1 . . -91.58(12) n
O10 Mo1 O5 Mo3 . . -174.68(13) n
O9 Mo1 O5 Mo3 . . -69.06(14) n
O4 Mo1 O5 Mo3 . . 56.4(2) n
O3 Mo1 O5 Mo3 . . 91.28(12) n
O1 Mo1 O5 Mo3 . . 16.88(10) n
O12 Mo3 O6 Na . . -163.37(14) n
O8 Mo3 O6 Na . . 93.11(15) n
O5 Mo3 O6 Na . . -64.26(16) n
O1 Mo3 O6 Na . . 8.73(15) n
O2 Mo3 O6 Na . . 42.1(4) n
O7 Na O6 Mo3 4_645 . 137.67(16) n
O9 Na O6 Mo3 . . 47.14(16) n
OW1 Na O6 Mo3 . . -55.20(16) n
O12 Na O6 Mo3 4_645 . -137.26(16) n
O11 Mo2 O7 Na . 4_655 153.45(17) n
O8 Mo2 O7 Na . 4_655 52.86(18) n
O4 Mo2 O7 Na 7_665 4_655 -103.54(17) n
O3 Mo2 O7 Na 7_665 4_655 -56.7(4) n
O2 Mo2 O7 Na . 4_655 -18.48(17) n
O6 Mo3 O8 Mo2 . . 177.07(13) n
O12 Mo3 O8 Mo2 . . 69.34(14) n
O5 Mo3 O8 Mo2 . . -55.4(2) n
O1 Mo3 O8 Mo2 . . -91.74(12) n
O2 Mo3 O8 Mo2 . . -16.90(10) n
O11 Mo2 O8 Mo3 . . -175.39(13) n
O7 Mo2 O8 Mo3 . . -69.43(14) n
O4 Mo2 O8 Mo3 7_665 . 54.9(2) n
O3 Mo2 O8 Mo3 7_665 . 92.11(12) n
O2 Mo2 O8 Mo3 . . 16.93(10) n
O10 Mo1 O9 Na . . 162.78(17) n
O4 Mo1 O9 Na . . -92.75(18) n
O5 Mo1 O9 Na . . 64.84(18) n
O3 Mo1 O9 Na . . -40.5(4) n
O1 Mo1 O9 Na . . -6.20(17) n
OW6 Na O9 Mo1 . . 132.98(18) n
O7 Na O9 Mo1 4_645 . -139.73(18) n
OW1 Na O9 Mo1 . . 32.5(2) n
O6 Na O9 Mo1 . . -48.48(18) n
O6 Mo3 O12 Na . 4_655 -153.45(16) n
O8 Mo3 O12 Na . 4_655 -52.23(18) n
O5 Mo3 O12 Na . 4_655 104.50(17) n
O1 Mo3 O12 Na . 4_655 51.0(4) n
O2 Mo3 O12 Na . 4_655 19.27(17) n
